Tunable Metal Oxide Frameworks via Coordination Assembly of Preyssler-Type Molecular Clusters.
Chen, Linfeng; San, Khin A.; Turo, Michael J.; Gembicky, Milan; Fereidouni, Shelir; Kalaj, Mark; Schimpf, Alina M.; Journal of the American Chemical Society  (2019) –; doi:10.1021/jacs.9b10277

data_4133772
_publ_section_title
;
 Tunable Metal Oxide Frameworks via Coordination Assembly of
 Preyssler-Type Molecular Clusters.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.9b10277
_journal_year                    2019
_chemical_formula_moiety
'0.13(K26.27 Na12 O1063.33 P40 W240 Zn27.68), 5.67(O), 0.15(Na)'
_chemical_formula_sum            'K3.28 Na1.65 O138.58 P5 W30 Zn3.46'
_chemical_formula_weight         8280.28
_space_group_crystal_system      orthorhombic
_space_group_IT_number           74
_space_group_name_Hall           '-I 2b 2'
_space_group_name_H-M_alt        'I m m a'
_audit_creation_date             2019-08-07
_audit_creation_method
;
Olex2 1.2-beta
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   52.137(3)
_cell_length_b                   21.5598(12)
_cell_length_c                   26.1562(16)
_cell_measurement_reflns_used    9899
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      25.97
_cell_measurement_theta_min      2.36
_cell_volume                     29401(3)
_computing_cell_refinement       'SAINT v8.38A (Bruker, 2017)'
_computing_data_collection       'APEX3 v2017.3-0 (Bruker, 2017)'
_computing_data_reduction        'SAINT v8.38A (Bruker, 2017)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      100.0
_diffrn_detector                 'Bruker APEX-II CCD'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'CCD Area Detector'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device       'Kappa Four-Circle Diffractometer'
_diffrn_measurement_device_type  'Bruker APEX II Ultra'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  'Double Bounce Multilayer Mirrors'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0793
_diffrn_reflns_av_unetI/netI     0.0468
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       64
_diffrn_reflns_limit_h_min       -63
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            114520
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         26.051
_diffrn_reflns_theta_min         1.224
_diffrn_source                   'Micro Focus Rotating Anode'
_diffrn_source_type              'Bruker Microstar FR-592'
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    24.175
_exptl_absorpt_correction_T_max  0.2598
_exptl_absorpt_correction_T_min  0.1220
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1353 before and 0.0830 after correction. The Ratio of minimum to maximum transmission is 0.4696. The \l/2 correction factor is Not present.'
_exptl_crystal_colour            'light white'
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    white
_exptl_crystal_density_diffrn    3.741
_exptl_crystal_description       octahedral
_exptl_crystal_F_000             28704
_exptl_crystal_size_max          0.042
_exptl_crystal_size_mid          0.027
_exptl_crystal_size_min          0.024
_refine_diff_density_max         3.447
_refine_diff_density_min         -4.716
_refine_diff_density_rms         0.599
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1102
_refine_ls_number_reflns         15064
_refine_ls_number_restraints     2085
_refine_ls_restrained_S_all      1.005
_refine_ls_R_factor_all          0.1220
_refine_ls_R_factor_gt           0.0887
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0846P)^2^+10568.8867P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2113
_refine_ls_wR_factor_ref         0.2452
_reflns_Friedel_coverage         0.000
_reflns_number_gt                11140
_reflns_number_total             15064
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja9b10277_si_006.cif
_cod_data_source_block           ZnImma
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_database_code               4133772
_shelx_shelxl_version_number     2016/6
_shelx_estimated_absorpt_t_max   0.631
_shelx_estimated_absorpt_t_min   0.361
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(K3) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O79) \\sim Ueq, Uanis(O6DA) \\sim Ueq, Uanis(O77) \\sim Ueq: with sigma
of 0.005 and sigma for terminal atoms of 0.01
Uanis(Na1) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(K2) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O6AA) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O15) \\sim Ueq, Uanis(O16) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
Uanis(O5BA) \\sim Ueq, Uanis(O4BA) \\sim Ueq: with sigma of 0.005 and sigma for
terminal atoms of 0.01
Uanis(O20) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O40) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(Zn4A) = Uanis(Zn4B)
Uanis(Zn1) = Uanis(Zn5)
Uanis(Zn3) = Uanis(Zn1)
Uanis(O43) = Uanis(O2BA) = Uanis(Zn4B) = Uanis(Zn4A)
Uanis(O81) = Uanis(O0CA)
2. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.002 and sigma for 1-3 distances of 0.002
3. Others
 Sof(Zn4A)=0.25*(1-FVAR(2))
 Sof(Zn4B)=0.25*FVAR(2)
 Fixed Sof: W14(0.5) W14B(0.5) W15(0.5) W15B(0.5) W16(0.5) Zn1(0.7) Zn2B(0.25)
 Zn2A(0.25) K0AA(0.2) K2B(0.5) P4(0.25) P4B(0.25) P5(0.25) P5B(0.25) P6(0.25)
 Na0A(0.25) Na2(0.25) O0CA(0.25) O2BA(0.25) O6DA(0.25) O37(0.5) O40(0.5)
 O41(0.5) O2B(0.5) O43(0.25) O44(0.5) O69(0.5) O70(0.5) O71(0.5) O72(0.5)
 O73(0.5) O74(0.5) O75(0.5) O76(0.5) O77(0.5) O79(0.5) O81(0.25) O82(0.5)
 O83(0.5) O84(0.5) O85(0.5) O86(0.5) O87(0.5) O78(0.25) O3AA(0.5) Na88(0.125)
 Na9(0.125) O1AA(0.125) O5AA(0.33333) O8AA(0.25) O9AA(0.75) O0BA(0.5)
 O3BA(0.33333) O6(0.33333) O4BA(0.5) O5BA(0.5) O6BA(0.5) O7BA(0.33333)
 O8BA(0.16667) Na1(0.075) K8(0.33333) O4AA(0.5) O6AA(0.16667)
;
_shelx_res_checksum              85169
_shelx_hkl_checksum              69845
_shelx_fab_checksum              74912
_platon_squeeze_void_probe_radius 1.20
_olex2_submission_special_instructions 'No special instructions were received'